Nonequilibrium spin-dependent phenomena in mesoscopic superconductor–normal metal tunnel
structures
Francesco Giazotto,1,
*
Fabio Taddei,1Pino D’Amico,1,2Rosario Fazio,1,3 and Fabio Beltram1 1_{NEST CNR-INFM and Scuola Normale Superiore, I-56126 Pisa, Italy}2_{Institut für Theoretische Physik, Universität Regensburg, D-93040 Regensburg, Germany} 3_{International School for Advanced Studies (SISSA), I-34014 Trieste, Italy}
共Received 1 June 2007; revised manuscript received 27 August 2007; published 20 November 2007兲
We analyze the broad range of spin-dependent nonequilibrium transport properties of hybrid systems com-posed of a normal region tunnel coupled to two superconductors with exchange fields induced by the proximity to thin ferromagnetic layers and highlight its functionalities. By calculating the quasiparticle distribution functions in the normal region, we find that they are spin dependent and strongly sensitive to the relative angle between exchange fields in the two superconductors. The impact of inelastic collisions on their properties is addressed. As a result, the electric current flowing through the system is found to be strongly dependent on the relative angle between exchange fields, giving rise to a huge value of magnetoresistance. Moreover, the current presents a complete spin polarization in a wide range of bias voltages, even in the quasiequilibrium case. In the nonequilibrium limit, we parametrize the distributions with an “effective” temperature, which turns out to be strongly spin dependent, though quite sensitive to inelastic collisions. By tunnel coupling the normal region to an additional superconducting electrode, we show that it is possible to implement a spin-polarized current source of both spin species, depending on the bias voltages applied.
DOI:10.1103/PhysRevB.76.184518 PACS number共s兲: 72.25.⫺b, 85.75.⫺d, 74.50.⫹r, 05.70.Ln
I. INTRODUCTION
Although the interest in nonequilibrium superconductivity dates back to the 1970s,1 _{nonequilibrium transport } phenom-ena in hybrid superconducting structures are currently under the spotlight. One of the key experiments that renewed this interest was probably the control of the supercurrent flowing through a Josephson junction, and even the reversal of its sign, accessible by altering the quasiparticle population in the weak link 共see Ref. 2 and references therein兲.
Out-of-equilibrium electron population can be realized in mesos-copic conductors subject to a bias voltage in which electrons cannot exchange energy either with one another or with lat-tice phonons, so that their energy distribution is not Fermi-like.3 _{Quasiequilibrium is reached if electrons can} thermalize, while still decoupled from the phonons, so that they can reach a temperature which is different from the one relative to the phonon bath. In ballistic Josephson junctions, supercurrent control occurs by inducing a nonequilibrium population of Andreev levels either by injecting a current through an additional normal terminal connected to the weak link4,5 _{or by applying an electromagnetic radiation on the} weak link.6,7 _{The} _{diffusive} _{long-junction} _{limit} _{was} considered8–11and experimentally realized too.12,13The con-trol of supercurrent by cooling electrons in the weak link was proposed in Refs.14–17and experimentally realized.18 _{It is} worthwhile stressing that electron temperature can be low-ered below the phonon temperature, thus realizing electron microrefrigeration,19,20_{by exploiting the superconducting } en-ergy gap共see Refs. 21and22and references therein兲.
Spin-dependent properties in out-of-equilibrium hybrid systems were investigated in a limited number of articles. In Refs. 23–26, ferromagnet-superconductor-ferromagnet double tunnel junctions were considered in order to study the spin imbalance induced in S by nonequilibrium. In the
anti-ferromagnetic alignment of the magnetizations of the F lay-ers, a strong suppression of superconductivity was found, leading to a large magnetoresistive effect. In Josephson junc-tions, the effect of spin injection27_{and the presence of weak} ferromagnets28were considered, while the effect of the An-dreev reflection on spin accumulation in a ferromagnetic wire was reported in Ref.29. In Ref. 30, the possibility of manipulating magnetism through the interplay of supercon-ductivity and nonequilibrium transport was investigated. Recently, we have proposed31 _{a hybrid } ferromagnet-superconductor共FS兲 spin valve whose operation is based on the interplay between out-of-equilibrium quasiparticle dy-namics and proximity-induced exchange coupling in super-conductors. Huge tunnel magnetoresistance values as high as several 106% has been predicted, leading to a fully tunable structure which shows high potential for application in spin-tronics. In this paper, we comprehensively investigate the physics and functionality of the setup analyzed in Ref.31, extending our study to the presence of finite electron-electron interaction and to the quasiequilibrium limit, as well as to the presence of nonidealities in the superconductors. In this setup, a spin-dependent “effective” temperature for the electrons in the N region emerges, thus leading to possible spin-dependent thermoelectric effects.
The paper is organized as follows. In Sec. II, we describe the system under investigation, and in Sec. III, we derive the quasiparticle distribution functions in different regimes. In particular, we consider the nonequilibrium limit in Sec. III A, we include the effect of inelastic collisions in Sec. III B, and we describe the quasiequilibrium regime in Sec. III C. In Sec. IV, we discuss the behavior of the electric current, fo-cusing on the magnetoresistive effects and on the spin-filtering properties of the system in Sec. V. Section VI is devoted to the characterization of the nonequilibrium distri-bution through an “effective” temperature and to the
tation of the system as a source of spin-polarized current through the introduction of an additional superconducting electrode. Finally, we draw our conclusions in Sec. VII.
II. SETUP
We consider a device consisting of two identical FS bi-layers共FS1,2兲 symmetrically connected to a mesoscopic
nor-mal metal region共N兲 of length t_{N}through tunnel contacts共I兲 of resistance Rt. The concentration of impurities is such that
quasiparticle transport is diffusive. The resulting system, a FS-I-N-I-SF heterostructure, is shown in Fig.1 in two dis-tinct experimental implementations. Figure 1共a兲 shows a spin-valve-like structure, which consists of a sequence of stacked metallic layers, while Fig.1共b兲displays a planar sys-tem. Although the two implementations are equivalent on theoretical footing, the planar configuration allows the mea-surement of local properties共e.g., the quasiparticle distribu-tion funcdistribu-tions as well as the local temperature兲 by connecting the N region to additional metallic probes. This will be ad-dressed in Sec. VI. For the sake of simplicity, we assume a symmetric system共a resistance asymmetry would not change the overall physical picture兲, tF 共tS兲 labels the F 共S兲 layer
thickness and a bias voltage V is applied across the structure. The exchange field in the left ferromagnet 共h1兲 is aligned
along the z axis for the setup in Fig.1共a兲or along the y axis for the setup in Fig.1共b兲, while that in the right F layer共h2兲
is misaligned by an angle关see Figs.1共a
⬘
兲 and1共b⬘
兲兴. Forsimplicity, we set兩h1兩=兩h2兩=h. In real structures, h2 can be
rotated by applying an in-plane magnetic field as low as some millitesla. Moreover, we assume that共i兲 the FS inter-face is transparent and 共ii兲 Rt is much larger than both the
resistance of the N layer共RN兲 and the FS contact resistance.
The first condition ensures that the superconductor is
strongly affected by the proximity of the F layer,32_{while the} second ensures that all the voltage drop occurs at the tunnel barriers共so that any spatial variation of the chemical poten-tial within the N region can be neglected兲 and that each FS bilayer is in local equilibrium.
The electronic properties of a FS bilayer can be analyzed within the quasiclassical Green’s function formalism.32 _{We} are interested in the situation in which the influence of the F layer on the superconductor becomes nonlocal. This occurs in the limit t_{S}⬍_{S}=
冑
បD/2kBTcand tF⬍F=冑
បD/h, whereSandFare the superconducting coherence length and the
length of condensate penetration into the ferromagnet, re-spectively. D denotes the diffusion coefficient, Tc is the
su-perconducting critical temperature, and kBis the Boltzmann
constant. In this situation, the ferromagnet induces in S a homogeneous effective exchange field共analogous to the one present in magnetic superconductors32_{兲 through proximity } ef-fect and modifies the superconducting gap共⌬兲. The effective values of the exchange field共h*兲 and gap 共⌬*兲 are given by33
⌬*_{/⌬ =}_{}
StS共StS+FtF兲−1,
h*/h =FtF共StS+FtF兲−1, 共1兲
whereS共F兲 is the normal-state density of states 共DOS兲 in S
共F兲. In particular, ifF=Sand for tFⰆtS, it follows that
⌬*_{/⌬ ⯝ 1,}
h*/h ⯝ tF/tSⰆ 1, 共2兲
i.e., h*turns out to be much smaller than in an isolated F layer. As a matter of fact, h*can take values of the order of magnitude of ⌬*. These conditions can be achieved quite easily in a realistic structure. We assume that the only effect of h* on the quasiparticles is to lead to a spin-dependent superconducting DOS, i.e., we neglect any influence of the induced magnetic moment on the orbital motion of electrons. Furthermore, we assume a negligible spin-orbit interaction.34 The superconductor DOS 共N_{}S兲 thus will be BCS-like but shifted by the effective exchange energy 共equivalent to that of a Zeeman-split superconductor in a magnetic field35兲. By choosing the spin quantization axis along the direction of the exchange field, we have
N_{}S_{共,h}*_{兲 =}1
2
冏
Re冋
+h*+ i⌫
冑
共 +h*+ i⌫兲2_{−}_{⌬}*2册
冏
, 共3兲where is the energy measured from the condensate chemi-cal potential,= ± 1 refers to the spin parallel 共antiparallel兲 to the direction of h_{1}, and⌫ is a smearing parameter.36 _{The} latter allows quasiparticle states within the gap due to inelas-tic scattering in the superconductor37 _{or inverse proximity} effect from the nearby metallic layers. Typical values for⌫ lie in the range⌫⬃1⫻10−5_{⌬, ... ,1⫻10}−3_{⌬ for Al as a }
thin-film superconducting electrode.36 _{In the following } calcula-tions, we set⌫=10−4⌬*, unless differently stated.
In order to describe our system, we make use of the tun-neling Hamiltonian approach and neglect proximity effects at NIS interfaces. F S1 N S2 F Rt Rt V/2 -V/2 tN x y z (a) tS tF (a’) z y h1 h2 φ N S1 S2 F F (b) tN Rt Rt (b’) y x h1 h2 φ V/2 -V/2
FIG. 1. 共Color online兲 Sketch of two possible implementations of the FS-I-N-I-SF structure analyzed in this work.共a兲 Spin-valve setup consisting of a sequence of stacked metallic layers. 共b兲 A planar structure. Ferromagnetic layers共F兲 induce in each supercon-ductor, through the proximity effect, an exchange field共h_{1,2}兲 whose relative orientation can be controlled by an externally applied mag-netic field. The F exchange fields are confined共a⬘兲 to the y-z plane for the setup shown in 共a兲 and 共b⬘兲 to the x-y plane for the setup shown in共b兲 and are misaligned by an angle. A voltage bias
V, applied across the structure, allows to control the energy
distributions in the N region. The structure is assumed quasi-one-dimensional.
III. QUASIPARTICLE DISTRIBUTIONS A. Negligible inelastic scattering: Full nonequilibrium limit
At finite bias V and in the limit of negligible inelastic scattering, quasiparticles in the N layer will be out of equi-librium and thus, in general, not distributed according to the Fermi function. The steady-state nonequilibrium distribution functions can be calculated by equating, at each energy value, the tunneling rate of quasiparticle entering the N re-gion from the insulating layer on the left-hand side to the tunneling rate of those exiting through the right-hand-side barrier.38_{In the general case of noncollinear exchange fields,} the spin eigenstates relative to S2 共兩↑典 and 兩↓典兲 can be
ob-tained by rotating the spin eigenstates relative to S1共兩⫹典 and
兩⫺典兲 by the angle共representing the misalignment between
h_{1} and h_{2}兲. As a consequence, spin up 共= + 1 with eigen-state兩⫹典兲 quasiparticles exiting the N layer through the right-hand-side barrier will now consist of two contributions. One describes tunneling into spin up 共with eigenstate 兩↑典兲 quasi-particles, proportional to cos2_{关}_{}_{/2兴, and the other describing}
tunneling into spin down共with eigenstate 兩↓典兲 quasiparticles, proportional to sin2_{关}_{}_{/2兴. As a result, the nonequilibrium}
distribution function in the N layer is spin dependent and can be written as f_{}共,V,h*,兲 =N S1FS1_{+}关a共兲N S2+ b共兲N − S2兴FS2 N_{}S1+ a共兲N tS2+ b共兲N − S2 , 共4兲
where a共兲=cos2关/2兴, b共兲=sin2关/2兴, FS1共S2兲
= f0共±eV/2兲, N_{}S1=NS共+eV/2兲, NS2=NS共−eV/2兲, f0共兲
is the Fermi function at bath temperature Tbath, and e is the
electron charge.
Figures2共a兲and 2共b兲 show the nonequilibrium distribu-tion funcdistribu-tions关calculated from Eq. 共4兲兴 for spin up and spin
down quasiparticles, respectively, vs energy for the parallel configuration共i.e.,= 0兲 at Tbath= 0.1Tc, h*= 0.2⌬*, and
dif-ferent values of V 共we assume the superconducting gap to follow the BCS relation⌬*= 1.764kBTc兲. Figure2shows that
by increasing the bias voltage V, spin up and spin down
distributions are shifted in opposite directions on the energy axis, similarly to what is expected in the presence of an effective spin-dependent chemical potential共_{}eff兲. In particu-lar, f+共兲 is shifted toward negative energies, while f−共兲
toward positive energies. Moreover, for eVⲏ⌬*, the spin-dependent chemical potential saturates at _{}eff= −h*. As shown in Ref.30, this effect can be used to electrostatically manipulate the magnetic properties of the N region. The role of a finite⌫ 共i.e., the presence of quasiparticle states within the gap兲 can be appreciated in Fig.2. By increasing eV from 0 to⌬*, the distributions broaden and reflect the heating of the N region, as discussed in Refs.22and36. This effect is absent for ⌫=0. By further increasing the bias voltage, the distribution functions sharpen due to cooling provided by the superconducting energy gap.22
Analogously, in Figs.3共a兲and3共b兲, we plot the nonequi-librium distribution functions for spin up and spin down qua-siparticles, respectively, for the antiparallel configuration 共i.e.,=兲. Distribution functions are shown vs energy for different values of V and were calculated for the same pa-rameters as in Fig.2. In this case, up and down distributions remain centered around =0 upon biasing 共equivalently, their effective chemical potential is always_{}eff= 0兲, but at a given bias voltage, the features of the distributions are more pronounced for the spin down case. As we shall see in Sec. VI, up and down distributions are characterized by different effective electronic temperatures 共T_{}eff兲. In general, for any angle differing from 0 or, the spin-dependent distribu-tion funcdistribu-tions f_{}共兲 will be characterized by both an effec-tive chemical potential and an effeceffec-tive electronic tempera-ture.
B. Intermediate inelastic scattering
In the presence of scattering, the approach of Sec. III A cannot be used and one has to resort to the kinetic equation theory. Electrons in metals experience both elastic and in-elastic collisions. The latter drive the system to equilibrium and can be expected to hinder the manifestation of the phe--1.0 -0.8 -0.6 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 0.0 0.5 1.0 0.0 0.5 1.0 _{eV = 0} 0.5∆∗ 1.0∆∗ 2.0∆∗ 2.5∆∗ f+ (ε ) T_{h}bath∗_{= 0.2}= 0.1T_{∆}∗ c φ= 0 (a) ε/∆∗ f− (ε ) (b)
FIG. 2.共Color online兲 Spin-dependent quasiparticle distribution functions f_{}共兲 in the full nonequilibrium limit vs energy for several bias voltages at=0, Tbath= 0.1Tc, and h*= 0.2⌬*.共a兲 f+共兲
and共b兲 f−共兲. -1.0 -0.8 -0.6 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 0.0 0.5 1.0 0.0 0.5 1.0 _{eV = 0} 0.5∆∗ 1.0∆∗ 2.0∆∗ 2.5∆∗ f+ (ε ) T_{h}∗bath_{= 0.2}= 0.1T_{∆}∗ c φ= π (a) ε/∆∗ f− (ε ) (b)
FIG. 3. 共Color online兲 Spin-dependent quasiparticle distribution functions f_{}共兲 in the full nonequilibrium limit vs energy for several bias voltages at=, Tbath= 0.1Tc, and h*= 0.2⌬*.共a兲 f+共兲
nomena discussed in the previous section. At low tempera-tures 共typically below 1 K兲, electron-electron scattering39 and scattering with magnetic impurities40,41are the dominant sources of inelastic collisions.3,41,42 _{Since R}
t is, in general,
large compared to the wire resistance 关RN= tN/共NFNe2DA兲兴,
whereN_{F}N is the N-region DOS at the Fermi energy and A the wire cross section兲, we can assume that f does not
de-pend on the position in the wire.15
In the following, we shall analyze the role of inelastic electron-electron relaxation on the quasiparticle distribution. The effect of electron-electron scattering due to the Coulomb interaction on the spin-dependent distributions can be ac-counted for by solving a pair of coupled stationary kinetic equations, D 2_{f} +共兲 x2 =Icoll + _{共兲,} D 2_{f} −共兲 x2 =Icoll − _{共兲,} _{共5兲}
together with the Kuprianov-Lukichev boundary conditions at the NIS interfaces.43_{In Eq.}_{共}_{5}_{兲, I}
coll
_{共兲 is the net collision}
rate at energy, functional of the distribution functions f_{}, defined by
Icoll 共兲 = Icollin共兲 − Icollout共兲, 共6兲
where
Icollin共兲 = 关1 − f共兲兴
冕
dk共兲
2 f共 −兲
冕
dE兵f+共E +兲 ⫻关1 − f+共E兲兴 + f−共E +兲关1 − f−共E兲兴其 共7兲and
Icollout共兲 = f共兲
冕
dk共兲
2 关1 − f共 −兲兴
冕
dE兵f+共E兲 ⫻关1 − f+共E +兲兴 + f−共E兲关1 − f−共E +兲兴其. 共8兲In Eqs.共7兲 and 共8兲, k共兲=ee−3/2according to the theory
of the screened Coulomb interaction44 _{for a } quasi-one-dimensional wire, whereee=共
冑
2Dប3/2NFNA兲−1.45,46 Byre-writing Eq.共5兲 in dimensionless units,15 _{the strength of the} electron-electron interaction can be expressed as Kcoll
=共Rt/RN兲共tN 2_{}
ee/D兲
冑
⌬=共tN/冑
2兲共Rt/RK兲冑
⌬/បD, where RK= h/2e2_{. We note that the strength of the electron-electron}
interaction turns out to be proportional to the length of the wire as well as to the tunnel barrier resistance.
We solved Eq. 共5兲 with h*= 0.2⌬*, eV =⌬*, and T = 0.1Tc for several Kcoll values.44,45 The effect of
electron-electron scattering on the quasiparticle distribution functions is displayed in Figs.4and5for= 0 and=, respectively. For the= 0 case, by increasing Coulomb interactions, the quasiparticle distributions are forced toward thermal ones still characterized by different chemical potentials for both spin species.30 _{In the antiparallel configuration} _{共see Fig.} _{5}_{兲,} the effect of inelastic relaxation is similar, but now the spin-dependent distribution function will coincide for sufficiently largeKcollvalues. It is easy to recognize that, in both cases,
a thermal Fermi-like distribution is reached for K_{coll} of the order of 10. Assuming parameters for a realistic Al/Al2O3/Ag SINIS microstructure21,36共with ⌬⯝200eV,
D = 0.02 m2_{s}−1_{, and R}
t= 1 k⍀兲, Kcoll= 10 corresponds to a
rather long N region, t_{N}⬇47m.
C. Strong inelastic scattering: Quasiequilibrium limit
This is the regime characterized by the fact that the electron-electron interaction is so strong that quasiparticles can reach an equilibrium共Fermi-like兲 distribution, while the electron-phonon coupling is negligible.22 _{Such distributions} are characterized by the quasiequilibrium chemical potential and temperature. Since electron-electron interaction occurs between quasiparticles irrespective of their spin 共in the ab-sence of spin-mixing mechanisms兲, the quasiequilibrium temperature 共Tqe_{兲 will be independent of spin and different}
from the temperature of the phonon bath Tbath. On the
con-trary, since electron-electron interaction redistributes the en-ergy among electrons of a given spin species, in the absence of spin-mixing mechanisms, the quasiequilibrium chemical potential 共_{}qe兲 will depend on the spin. This is a
conse--1.0 -0.8 -0.6 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 -1.0 -0.8 -0.6 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 -1.0 -0.8 -0.6 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 -1.0 -0.8 -0.6 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 0.0 0.0 0.0 0.0 0.5 0.5 0.5 0.5 1.0 1.0 1.0 1.0 0.0 0.0 0.0 0.0 0.5 0.5 0.5 0.5 1.0 1.0 1.0 1.0 _{K}_{K}_{K}_{K} coll coll coll coll= 0= 0= 0= 0 0.01 0.01 0.01 0.01 0.1 0.1 0.1 0.1 1.0 1.0 1.0 1.0 10 10 10 10 fff f++++ ((( ( εεε ε ))) ) TTT
Tbathbathbathbath= 0.1= 0.1= 0.1= 0.1TTTTcccc
hhh h∗∗∗∗ = 0.2 = 0.2 = 0.2 = 0.2∆∆∆∆∗∗∗∗ eV eV eV eV= 1.0= 1.0= 1.0= 1.0∆∆∆∆∗∗∗∗ φφφ φ= 0= 0= 0= 0 (a) (a) (a) (a) εεε ε////∆∆∆∆∗∗∗∗ fff f−−−− ((( ( εεε ε ))) ) (b) (b) (b) (b)
FIG. 4. 共Color online兲 Spin-dependent quasiparticle distribution functions f_{}共兲 vs energy calculated for several K_{coll}values at =0, eV=⌬*_{, T}
bath= 0.1Tc, and h*= 0.2⌬*.共a兲 f+共兲 and 共b兲 f−共兲.
-1.0 -0.8 -0.6 -0.4 -0.2 0.0 0.2 0.4 0.6 0.8 1.0 0.0 0.5 1.0 0.0 0.5 1.0 _{K} coll= 0 0.01 0.1 1.0 10 f+ (ε ) T_{bath}= 0.1T_{c} h∗_{= 0.2}_{∆}∗ eV = 1.0∆∗ φ= π (a) ε/∆∗ f− (ε ) (b)
FIG. 5. 共Color online兲 Spin-dependent quasiparticle distribution functions f_{}共兲 vs energy calculated for several K_{coll}values at =, eV=⌬*_{, T}
quence of the fact that the number of electrons of a given spin must be conserved. Furthermore, both quasiequilibrium chemical potential and quasiequilibrium temperature will de-pend on; therefore, they will be different for parallel and antiparallel configurations.
In the absence of spin-flip mechanisms, the quasiequilib-rium distribution functions can be calculated by imposing the conservation of particle currents, independently for the two spin species, together with a balance equation for the heat currents. In particular, in the former case, we require that
I_{}L共V,h*,兲 = I_{}R共V,h*,兲, 共9兲 where I_{}L共V,h*,兲 = 1 eRt
冕
dN_{}S1共兲关FS1共兲 − f 共兲兴 共10兲 and I_{}R共V,h*,兲 = 1 eR_{t}冕
d关N S2共兲a共兲 + N − S2共兲b共兲兴关f 共兲 −FS2共兲兴 共11兲are the electric currents flowing through the left共L兲 and right 共R兲 NIS interface. Note that in contrast to the full nonequi-librium regime where the tunneling rates are set to be equal at each energy, here the conservation involves the total cur-rents since the electron-electron interaction mixes the energy of the electrons. In the absence of electron-phonon coupling, the only contribution to the heat flux is the heat current flow-ing off the N region through each NIS interface. The latter is given by
J_{}L共V,h*,兲 = 1 e2Rt
冕
dN_{}S1共兲关f
共兲 − FS1共兲兴, 共12兲
for the left NIS contact, and by
J_{}R共V,h*,兲 = 1 e2Rt
冕
d关N_{}S2共兲a共兲 + N − S2共兲b共兲兴 ⫻关f共兲 − FS2共兲兴, 共13兲for the right contact. The balance equation for the heat flux thus simply reads
兺
_{} 关J_{}L_{共V,h}*_{,}_{}_{兲 + J} R_{共V,h}*_{,}_{}_{兲兴 = 0.} _{共14兲}
By assuming that f_{}= f0共−qe, Tqe兲 and solving Eqs. 共9兲
and 共14兲, the temperature and chemical potentials can be
easily determined. It turns out that while in the antiparallel alignment spin up and down distributions are equal, in the parallel one, the two spin components have equal effective electronic temperature共though different from the antiparallel alignment兲 but opposite effective chemical potential 共see Figs.4and5for largeKcollvalues兲. Although the
quasiequi-librium regime might seem an unrealistic limit, it actually describes the case of a strong electron-electron interaction quite well. Indeed, according to our calculations共Sec. III B兲, quasiequilibrium distributions are already reached for an electron-electron collision strengthKcoll⯝10. In the
follow-ing sections, we shall investigate the impact of quasiequilib-rium on spin-dependent transport properties.
IV. ELECTRIC CURRENT
The transport properties of the FS-I-N-SF structure are determined by the spin-dependent distribution functions f_{}. We note that although a Josephson current can flow through the system, its theoretical description is beyond the scope of the present paper. As a matter of fact, we shall be only con-cerned with the quasiparticle transport. Furthermore, al-though similar results for tunnel magnetoresistance and cur-rent polarization could be obtained in a FS-I-SF structure 共i.e., without the N interlayer兲 and not relying on nonequi-librium, the present system possesses a crucial advantage. In fact, a FS-I-SF structure implies an additional undesired Jo-sephson current, which can be fairly large as compared to the quasiparticle current 共around 1 order of magnitude larger than the quasiparticle current relevant for high tunnel mag-netoresistance and current polarization, see, for example, Ref. 33兲. Such supercurrent could be suppressed, for
in-stance, by the application of an additional in-plane magnetic field. This field, however, would largely exceed that required to control the orientation of h*. By contrast, in the FS-I-N-I-SF system, the supercurrent can be kept extremely small up to a large extent, depending mainly on t_{N}, on the tunnel barrier transmissivity, and on the N-interlayer material pa-rameters. A simple estimate for the Josephson coupling in our structure reveals that the supercurrent can be from 1 to several orders of magnitude smaller than the quasiparticle current共see, for example, Ref.47兲.
The quasiparticle current I共e.g., evaluated at the left in-terface兲 is given by
I共V,h*,兲 =
兺
I_{}L共V,h*,兲. 共15兲 Figure 6共a兲displays the electric current in full nonequilib-rium vs bias voltage V calculated for several angles at h*= 0.2⌬*and T = 0.1Tc. A sizable current starts to flow only
when the voltage V is such that the DOS is finite for both superconductors in some range of energies. For = 0, the current rises sharply at兩eV兩=2⌬*, similarly to the quasipar-ticle current of a SIS junction 共also in the presence of an in-plane magnetic field35_{兲. In this case, in fact, the DOS of a} given spin is shifted by the Zeeman energy in the same di-rection for both superconductors. In contrast, for=, cur-rent sets off at兩eV兩=2共⌬*− h*兲.
Figure6共b兲shows the nonequilibrium differential conduc-tance
G共V,h*,兲 =dI共V,h
*_{,}_{}_{兲}
dV , 共16兲
calculated for the same values as in Fig. 6共a兲. Additional features are present at兩eV兩=2h*, which are strongly tempera-ture dependent and vanish in the limit T→0 共the zero-bias conductance peak for⫽ resembles that typical of a SIS junction composed of identical superconductors48_{兲. These are} a consequence of the overlapping of the superconducting
DOSs where only thermally activated quasiparticles exist at finite temperature.
All these simply reflects how the spin-dependent DOS in each superconductor contributes to the total quasiparticle current at different V. This can be easily visualized by in-specting Fig.7, which shows idealized finite-temperature ex-change field-split superconducting DOS for parallel spin spe-cies, at different bias voltages V and for the case =. In this case, the DOS of S_{1} is shifted in the opposite direction with respect to that of S2 关see Fig.7共a兲for V = 0兴. Then, by
biasing the structure, the required voltage for a current to flow is smaller with respect to the = 0 case, i.e., eV = 2共⌬*_{− h}*_{兲 关see Fig.} _{7共b兲}_{兴. In the same way, for negative}
voltages, the current sets off at eV = −2共⌬*_{+ h}*_{兲, as shown in}
Fig. 7共d兲. It is also clear that antiparallel spin species will give rise to features at the opposite bias voltage, therefore explaining the origin of additional feature appearing at eV = 2共⌬*_{+ h}*_{兲. For intermediate values of} _{}_{, features are}
present at兩eV兩=2共⌬*± h*兲 and at 兩eV兩=2⌬*since contribu-tions from both= 0 and=configurations are present. Of particular relevance is the voltage interval 2共⌬*− h*兲艋兩eV兩 艋2⌬*_{. By increasing}_{}_{from 0 to}_{}_{, the current is enhanced}
from a vanishingly small value up to a finite value leading to a spin-valve effect.
It is noteworthy to mention that the nonequilibrium con-dition is essential for the observation of the spin-valve effect. At equilibrium, the distribution functions in the N layer would be thermal and spin independent.
V. MAGNETORESISTANCE
The spin-valve properties of the FS-I-N-I-SF setup can be evaluated quantitatively by analyzing the tunnel magnetore-sistance ratio共TMR兲, defined as
TMR共V,h*_{,}_{}_{兲 =}G共V,h*,兲 − G共V,h*,0兲
G共V,h*,0兲 . 共17兲 Figure8共a兲displays the absolute value of the nonequilibrium
0.0 0.5 1.0 1.5 2.0 2.5 3.0 0.00 0.25 0.50 0.75 -0.5 -0.4 -0.3 -0.2 -0.1 0.0 0.1 0.2 0.3 0.4 0.5 5.5 6 6.5 7 7.5 8 2(∆∗_{-h}∗_{)} eR t I/ ∆ ∗ eV/∆∗ φ= 0 π/4 π/2 3π/4 π Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ (a) 2(∆∗_{+h}∗_{)} -2h∗ Rt G eV/∆∗ φ= 0 π/4 π/2 3π/4 π Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ (b) 2h∗ x10-5
FIG. 6. 共Color online兲 共a兲 Nonequilibrium current vs bias volt-age V for several angles at T_{bath}= 0.1T_{c}and h*= 0.2⌬*.共b兲 Non-equilibrium differential conductance G vs V calculated for the same values as in共a兲. 0 ∆∗ -∆∗ ε S1(ε) eV = -2h∗∗∗∗ h∗ S2(ε) ε -∆∗ 0 _{∆}∗ h∗ 0 ∆∗ -∆∗ ε S1(ε) eV = -2(∆∆∆∆∗∗∗∗_{+h}∗∗∗∗_{)} h∗ S2_{(ε)} ε h∗ 0 ∆∗ -∆∗ h∗ 0 ∆∗ -∆∗ ε S1_{(ε)} eV = 0 S2_{(ε)} ε -∆∗ _{0} _{-∆}∗ h∗ h∗ 0 ∆∗ -∆∗ ε S1_{(ε)} eV = 2(∆∆∆∆∗∗∗∗_{-h}∗∗∗∗_{)} S2_{(ε)} ε h∗ -∆∗ _{0} _{∆}∗
φ
=
π
(a) (c) (d) (b)FIG. 7. 共Color online兲 Idealized finite-temperature exchange field-split density of statesNS1,2_{of S}_{1,2}_{for parallel spin species, at}
= and different bias voltages V. In particular, 共b兲, 共c兲, and 共d兲 show how features in the tunneling current originate at eV = 2共⌬* − h*兲, eV=−2h*, and eV = −2共⌬*+ h*兲, respectively. Antiparallel spin species gives rise to features at opposite voltages. Green-dashed lines represent the superconducting DOS in the absence of the exchange field.
10-1 101 103 105 107 -3 -2 -1 0 1 2 3 10-1 101 103 105 107 2(∆∗_{+h}∗_{)} φ=π/16 π/8 π/4 π/2 π |T M R |( %) Tbath= 0.1Tc h* = 0.2∆* 2h∗ 2(∆∗_{-h}∗_{)} (a) h∗_{= 0.4}_{∆}∗ 0.3∆∗ 0.2∆∗ 0.1∆∗ eV/∆∗ |T M R |( %) (b) T_{bath}= 0.1T_{c} φ= π
FIG. 8. 共Color online兲 共a兲 Nonequilibrium tunnel magnetoresis-tance ratio 兩TMR兩 vs V calculated for several angles at Tbath
= 0.1T_{c} and h*= 0.2⌬*. 共b兲 兩TMR兩 vs V for different h* values at
TMR vs bias voltage V calculated for several anglesat T = 0.1Tcand h*= 0.2⌬*. For 2共⌬*− h*兲艋兩eV兩艋2⌬*, the TMR
increases monotonically by increasingand is maximized at
=where it reaches huge values exceeding 106_{%. We note}
that in the limit T = 0 and⌫=0, 兩TMR兩 diverges, realizing an ideal full spin-valve effect. The nonequilibrium TMR behav-ior for several exchange field values is shown in Fig.8共b兲, at T = 0.1Tc and=. By decreasing h*, the maximum TMR
value reduces and so does the voltage interval of larger mag-netoresistance. Larger h*values are thus preferable in order to extend the voltage window for optimized operation and to maximize the TMR.
The spin-filtering properties of this system can be quanti-fied by inspecting the current polarization共PI兲, defined as
PI共V,h*,兲 =
I_{+}L共V,h*,兲 − I_{−}L共V,h*,兲
I_{+}L共V,h*,兲 + I_{−}L共V,h*,兲. 共18兲 The calculated nonequilibrium PI vs V is displayed in Fig. 9共a兲for several values, at T = 0.1Tc and h*= 0.2⌬*. Upon
increasing, two intervals of 100% spin-polarized current develop for 2共⌬*− h*兲艋兩eV兩艋2⌬*, extending to wider re-gions关2共⌬*− h*兲艋兩eV兩艋2共⌬*+ h*兲兴 asapproaches. For
= 0, PIvanishes like in SIS junctions with an in-plane
mag-netic field.35_{Depending on bias, fully spin-polarized currents} of both parallel and antiparallel spin species can be obtained. The structure can thus also be operated as a controllable spin filter by changing the orientation of h_{2}as well as by varying V. Figure9共b兲shows PI vs V for several h*at T = 0.1Tcand
=. The net effect of increasing h*is to widen the regions of 100% spin-polarized current.
It is important to discuss the effect of the smearing pa-rameter⌫ 共which controls the presence of quasiparticle states within the superconducting gap兲 on the magnetoresistance
and current polarizations. As shown in Fig.10共a兲, by increas-ing⌫, the TMR value decreases mostly in the region 2共⌬* − h*兲艋兩eV兩艋2⌬*, while for other values of V, almost no changes are found apart from some smoothing of sharp fea-tures. In particular, the normal character of transport is strengthened by increasing⌫, which causes a suppression of the large TMR value. The latter, indeed, is a consequence of the presence of the superconducting gap. On the contrary, the impact of⌫ on PI, plotted in Fig.10共b兲as a function of the
voltage V, is much weaker: the polarization in the range 2共⌬*− h*兲艋兩eV兩艋2共⌬*+ h*兲 is almost insensitive to ⌫, be-ing slightly reduced only for⌫ values as large as 10−2_{⌬}*_{.}
TMR values are expected to be marginally affected by the presence of electron-electron relaxation in the N layer. In-deed, as discussed in Secs. III B and III C, Coulomb interac-tion allows quasiparticles to exchange energy 共through in-elastic collisions兲 without coupling the two spin species. As shown in Figs.4 and 5, inelastic scattering leaves the two distributions f+共兲 and f−共兲 strongly spin dependent in the
parallel configuration, while making them to coincide in the antiparallel configuration, so that both magnetoresistance and current polarizations are expected to be only slightly af-fected. Indeed, TMR is only marginally affected even in the quasiequilibrium regime, as shown in Fig. 11共a兲, where we compare TMR at=, as a function of V, for the full non-equilibrium and the quasinon-equilibrium regimes. The effect of energy redistribution characteristic of quasiequilibrium con-sists merely in a smoothing of some of the sharp features present in the nonequilibrium limit. In Fig. 11共b兲, we com-pare the plots of PI at = as functions of V for both
re-gimes. In particular, quasiequilibrium displays a reduction of polarization for兩V兩⬎2共⌬*− h*兲 and an increase of polariza-tion for兩V兩 ⬍2共⌬*− h*兲. Nevertheless, PI values as large as
100% can be obtained in the quasiequilibrium limit as well. -100 -50 0 50 100 -4 -3 -2 -1 0 1 2 3 4 -100 -50 0 50 100 Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ PI (% ) φ = π/16 π/4 π/2 3π/4 π φ= 0 (a) h∗_{= 0.4}_{∆}∗ 0.3∆∗ 0.2∆∗ 0.1∆∗ 0.01∆∗ eV/∆∗ PI (% ) (b) Tbath= 0.1Tc φ=π
FIG. 9. 共Color online兲 共a兲 Nonequilibrium current polarization
PI vs V calculated for several angles at Tbath= 0.1Tc and h* = 0.2⌬*. 共b兲 P_{I} vs V for different h* values at T_{bath}= 0.1T_{c}and =. -3 -2 -1 0 1 2 3 -100 -50 0 50 100 10-1 101 103 105 107 109 Γ= 10-6 ∆∗ 10-5_{∆}∗ 10-4_{∆}∗ 10-3 ∆∗ 10-2 ∆∗ |TMR |(%) Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ φ= π (a) Γ= 10-6_{∆}∗ 10-5_{∆}∗ 10-4 ∆∗ 10-3 ∆∗ 10-2_{∆}∗ eV/∆∗ PI (% ) (b) Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ φ= π
FIG. 10. 共Color online兲 共a兲 Nonequilibrium tunnel magnetore-sistance ratio兩TMR兩 vs V calculated for several ⌫ values at Tbath
= 0.1T_{c}, h*= 0.2⌬*, and=. 共b兲 Nonequilibrium P_{I} vs V calcu-lated for the same values as in共a兲.
The full evolution of PI as a function of Kcollin the
rel-evant intervals of large polarization is shown in Figs.11共c兲
and11共d兲. It is easy to notice the gradual smearing of PI by
increasing the electron-electron interaction strength, and that the quasiequilibrium limit is already reached for K_{coll}⬃10 共see also the discussion at the end of Sec. III B兲. However, in FS-I-N-I-SF realistic structures, it should be possible to keep Kcoll⬃0.1 or smaller so that current polarization would be
somewhat similar to that obtained in the full nonequilibrium limit.
By contrast, TMR must decrease if spin-flip processes mix the spin-dependent distributions. In metals and at low temperature共typically below ⬃1 K兲, such processes are nor-mally caused by the presence of magnetic impurities in the N layer. Spin-flip scattering can be suppressed by limiting the magnetic-impurity content in the N layer and by choosing tNⰆsf关the spin-flip relaxation length sfis of the order of
some micrometers in metals such as Cu or Au共Refs.49and
50兲兴. These constraints can be met fairly easily
experimen-tally in multilayered or planar structures like the ones pre-sented here.
VI. SPIN-DEPENDENT EFFECTIVE TEMPERATURE
Even in the nonequilibrium case, it is interesting to char-acterize the distribution function through an effective tem-perature and an effective chemical potential. Such effective quantities can be meaningfully defined by fictitiously con-necting the N region to a large normal metal reservoir through an insulating barrier that is sufficiently transparent to allow the flow of quasiparticles but opaque enough not to alter the nonequilibrium condition of the electrons. One can identify the effective chemical potential共_{}eff兲 of the out-of-equilibrium electron gas in the N region with the chemical potential the reservoir must possess in order for the particle current to be zero. The effective temperature 共T_{}eff兲, on the other hand, is taken to be equal to the one the reservoir must have in order for the heat current to be zero.51_{These } condi-tions can be expressed by the following two equacondi-tions:
冕
d关f_{}共兲 − f0共 −eff,Teff兲兴 = 0, 共19兲冕
d关f_{}共兲 − f0共 −eff,Teff兲兴 = 0, 共20兲where we have assumed that the DOS of the N reservoir is equal to that of the N layer. We wish to warn the reader that the words “temperature” and “chemical potential” have to be taken in a loose sense, especially when the distributions are very different from equilibrium functions. They are merely two parameters which grasp important characteristic proper-ties of the distributions, related, namely, to particle and heat transport.
A general expression for the effective temperature can be easily derived through the Sommerfeld expansion,36 _{} obtain-ing T_{}eff=
冑
6 kB冑
冕
_{−⬁} ⬁ d关f_{}共兲 − f_{0}共 −_{}eff,T = 0兲兴, 共21兲 where _{}eff_{=}冕
−⬁ ⬁ d关f_{}共兲 −共兲兴, 共22兲 and共兲 is the Heaviside step function. Equation 共21兲 yieldsthe true spin-dependent electron temperature in 共quasi兲equi-librium. Furthermore, in the present FS-I-N-I-SF system, T_{}eff turns out to depend on the strength of electron-electron in-teraction 共i.e., on Kcoll兲 as we shall show in the following,
due to heat exchange with FS reservoirs with nonconstant DOS.22,36
In Figs.12共a兲and12共b兲, we plot the calculated effective temperatures in the full nonequilibrium limit 共i.e., for Kcoll
= 0兲, normalized with respect to the bath temperature 共Tbath
= 0.1Tc兲, as a function of the applied bias voltage V for
= 0 and =, respectively. In the former case, there is no spin dependence and T_{±}eff is an even function of the bias voltage. Starting from the equilibrium condition 共i.e., at V = 0 where the T_{±}eff= T_{bath}兲, the temperature first increases reaching a maximum around eV/⌬*_{= 0.8 and thereafter }
de--3 -2 -1 0 1 2 3 -100 -50 0 50 100 1.5 2.0 2.5 3.0 -100 -80 -60 -40 -20 0 -3.0 -2.5 -2.0 -1.5 0 20 40 60 80 100 10-1 101 103 105 107 nonequilibrium quasiequilibrium |T M R | (%) Tbath= 0.1Tc h∗ = 0.2∆∗ φ = π (a) nonequilibrium quasiequilibrium eV/∆∗ PI (% ) (b) T_{bath}= 0.1Tc h∗ = 0.2∆∗ φ = π T_{bath}= 0.1T_{c} h∗ = 0.2∆∗ φ = π eV/∆∗ (d) n.e 0.01 0.1 1 5 10 q.e. eV/∆∗ PI (% ) (c) K_{coll}
FIG. 11. 共Color online兲 共a兲 Tunnel magnetoresistance ratio 兩TMR兩 vs V in nonequilibrium 共solid line兲 and quasiequilibrium 共dash-dotted line兲 at Tbath= 0.1Tc, h*= 0.2⌬*, and=. 共b兲 Current polarization PI vs V in nonequilibrium共solid line兲 and quasiequi-librium共dash-dotted line兲 calculated for the same values as in 共a兲. 关共c兲 and 共d兲兴 PIvs V in the intervals of large polarization calculated for severalKcollvalues and the same parameters as in共a兲.
creases down to the minimum around eV/⌬*_{= 2. The initial}
increase is the “anomalous heating” due to the presence of a finite DOS within the superconducting gap,22,36 _{while the} minimum reflects the usual electron “cooling,” which is maximized for voltages around twice the value of the gap22 共see the discussion in Sec. III A兲. Such features are present also in the absence of an exchange field, with negligible quantitative differences. By contrast, the effect of the ex-change field is manifested in the antiparallel configuration. Indeed, the effective temperatures are different for the two spin species, though related according to the relation T_{}eff共−V兲=T_{−}eff共V兲. In particular, minima are shifted by an amount equal to 2h*toward higher共lower兲 voltages for spin up 共down兲 electrons. This fact can also be understood through the schemes shown in Fig. 7, as due to the shift, introduced by the exchange field, of the DOS of the two superconductors in opposite directions. For spin up electrons, maximum cooling occurs for eV = 2共⌬*_{− h}*_{兲 关see Fig.} _{7共b兲}_{兴}
and for eV = −2共⌬*_{+ h}*_{兲 关see Fig.}_{7共d兲}_{兴. For spin down }
elec-trons, maximum cooling occurs at opposite voltages. The position and amplitude of maxima turns out to be a function of the exchange field, as well as of the smearing parameter⌫. Notably, as shown in Fig.12共b兲, the spin-dependent effective temperatures can be largely different upon voltage biasing the structure.
In Fig. 13共a兲, we plot the nonequilibrium effective tem-perature difference ␦Teff_{= T}
+ eff_{− T}
−
eff _{normalized to the bath}
temperature共Tbath= 0.1Tc兲 versus V at=and for different
values of the exchange field h*. ␦Teffis odd in the applied voltage and is more pronounced for larger values of h*. For positive values of V, the maximum共as large as 500% at this bath temperature兲 corresponds to the anomalous heating 共oc-curring around eV/⌬*_{⯝1兲, while the minimum occurs for}
eV/⌬*ⲏ2 and moves to higher values as h*increases. The effect of electron-electron inelastic collisions is ad-dressed in Fig.13共b兲, which shows␦Teff_{/T}
bath at=as a
function of the collision strength K_{coll} for eV = 1.0⌬*, h* = 0.2⌬*_{, and T}
bath= 0.1Tc. We find a dramatic effect of
electron-electron interaction that leads to a strong suppres-sion of the effective temperature difference on the scale of
Kcoll⯝0.1. With the material parameters given in Sec. III B,
this would correspond to a N region with t_{N}⬇470 nm. The possibility to have access to different spin-dependent electronic temperatures suggests that we investigate the po-tential for the implementation of spintronic devices. In par-ticular, we conceive a nanostructure like that shown in Fig.
14共a兲, where an additional voltage-biased superconducting electrode 共S3兲 is tunnel coupled to the N region through a
junction of resistance RpⰇRt,52 while the exchange fields in
S1,2 are arranged in the antiparallel configuration 共=兲.
The presence of a superconducting extraction lead is crucial since in the tunneling process, the quasiparticle current through S_{3} will depend exponentially on the electron tem-perature in N.22 _{On one hand, the setup considered allows} direct measurement of the spin-dependent electron tempera-tures and S3may act as a thermometer.22S3provides, in fact,
access to the whole distribution functions f_{}共兲 from the voltage-dependent differential conductance of the NIS_{3} junction.3_{On the other hand, upon biasing the S}
3 electrode
with Vbias, the existence of different spin-dependent
tempera-tures in the normal metal region yields a finite current polar-ization PI defined in the usual way as
PI共V,Vbias,h*兲 = I_{+}S3共V,V bias,h*兲 − I− S3共V,V bias,h*兲 I_{+}S3共V,V bias,h*兲 + I− S3共V,V bias,h*兲 , 共23兲 where I_{}S3共V,V bias,h*兲 = 1 eRp
冕
dNS3共 + eV bias兲关f共,V,h*兲 − f0共 + eVbias兲兴, 共24兲andNS3共兲 is the normalized DOS of S
3. In the following,
we assume for simplicity thatNS3共兲 is identical to the
den--3 -2 -1 0 1 2 3 0 2 4 6 0 2 4 6 σ= + -T eff /T_{σ} ba th Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ φ= 0 (a) σ= + -eV/∆∗ T ef f σ /Tba th (b) Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ φ= π
FIG. 12.共Color online兲 共a兲 Nonequilibrium spin-dependent elec-tron effective temperature T_{}eff vs V calculated for =0 at Tbath
= 0.1Tc and h*= 0.2⌬*. 共b兲 T_{}effvs V calculated for = at Tbath
= 0.1Tcand h*= 0.2⌬*. 0.00 0.02 0.04 0.06 0.08 0.10 0 1 2 -3 -2 -1 0 1 2 3 -10 -5 0 5 10 h∗_{= 0.4}_{∆}∗ 0.3∆∗ 0.2∆∗ 0.1∆∗ eV/∆∗ δ T eff /T ba th T_{bath}= 0.1T_{c} φ=π (a) h∗_{= 0} K_{coll} δ T ef f /T ba th (b) Tbath= 0.1Tc h∗_{= 0.2}_{∆}∗ eV = 1.0∆∗ φ=π
FIG. 13. 共Color online兲 共a兲 Difference of the nonequilibrium spin-dependent electron effective temperatures␦Teff_{vs V calculated}
for different h*values at Tbath= 0.1Tc and=. 共b兲␦TeffvsKcoll calculated at eV = 1.0⌬*for T_{bath}= 0.1T_{c}, h*= 0.2⌬*, and=.
sity of states of S1,2in the absence of an exchange field共i.e.,
h*= 0兲.
Figure14共b兲shows the calculated nonequilibrium PIas a
function of V and Vbias, for Tbath= 0.1Tcand h*= 0.2⌬*. For
easily attainable values of V and Vbias, pure共i.e., 100%兲
spin-polarized current of both the parallel and antiparallel spin species can be achieved. Furthermore, we note that 兩PI兩
largely exceeds 50% over a wide region in the 共V,Vbias兲
plane. It is worthwhile to note that replacing the S3terminal
with a N metal reservoir would completely hinder the extrac-tion of a finite spin-polarized current for =. This stems from the insensitivity of the tunneling current in a NIN junc-tion to the N-region temperature. The= 0 case for a N lead connected to a similar setup was analyzed in Ref.30.
The role of electron-electron inelastic relaxation is dis-played in Fig. 14共c兲, which shows PI versus Kcoll at eV
=⌬* and eVbias= 0.5⌬*, for Tbath= 0.1Tc and h*= 0.2⌬*. We
find that the suppression of the current polarization occurs on a larger range of values ofKcollwith respect to the electron
effective temperature difference关note the different scale for the horizontal axis of Figs.13共b兲 and14共c兲兴. At Kcoll= 0.1,
for example, PIis reduced only by about 35%. This behavior
is not surprising: it originates, as mentioned above, from the
fact that the current extracted from S3 is exponentially
sen-sitive to T_{}eff. As a consequence, even a small temperature difference between spin species yields a large current differ-ence and gives rise to a sizable PIvsKcollcharacteristic.
We shall further comment the impact of relaxation in this setup as compared to that of Fig.1by inspecting Figs.14共c兲
and11共b兲–11共d兲. In particular, they show that while electron-electron interaction is crucial in suppressing PIin the former
case, it is much less important in the setup of Fig.1. The reason stems from the fact that while in the present case the electric current is spin dependent only, thanks to the presence of spin-dependent distribution functions in the N region关as expressed by Eq.共24兲兴, in the setup of Fig.1, the spin selec-tivity originates from both the distribution functions f_{} and the spin-dependent superconducting DOS关see Eqs. 共10兲 and
共11兲兴. From this it follows that, in the first setup, current
polarization will completely vanish at quasiequilibrium 共where the quasiparticle distribution functions result to be identical and spin independent兲, while in the second system, spin polarization will persist also for identical thermal distri-bution functions owing to the additional spin selectivity pro-vided by spin-split DOS in the superconductors.
VII. CONCLUSIONS
In this paper, we have analyzed the nonequilibrium spin-dependent transport properties in superconductor–normal metal tunnel nanostructures, where the superconductors present a proximity-induced effective exchange field 共equivalent to that of a superconductor in a magnetic field兲. The latter is due to the proximity of a ferromagnetic thin layer which exerts, under appropriate conditions, a nonlocal influence. We have computed the quasiparticle distributions of a normal metal layer tunnel coupled to two superconduct-ors with noncollinear exchange fields. In the full nonequilib-rium limit, i.e., in the absence of any inelastic relaxation mechanisms, the distribution functions depend on the spin and display unusual features, such as population inversion and double-step shape, depending on the bias voltage applied to the superconductors. Spin dependence persists also in the presence of inelastic Coulomb interaction, which produces a smoothing of the sharp features and tends to drive electrons into the quasiequilibrium regime, where the energy relax-ation is strong enough to allow electrons to thermalize. This interesting behavior is reflected in the current-voltage char-acteristic, which shows a strong dependence on the relative orientation of the exchange fields existing in the supercon-ductors. Notably, even in the quasiequilibrium regime, a huge tunnel magnetoresistance ratio and a complete current spin polarization were found over a wide range of bias volt-ages and for realistic parameters. The impact of the exchange field as well as of the presence of subgap states in the DOS of the superconductors have been addressed.
We have characterized the out-of-equilibrium distribution functions through an “effective temperature” and an “effec-tive chemical potential,” defined in an opera“effec-tive sense. We have found that such effective temperatures are strongly spin dependent for antiparallel exchange fields, the relative tem-perature difference being as high as 500%. Furthermore, we x y z N S1 S2 F F (a) V/2 -V/2 y x h1 h2 φ = π A Vbias Rp S3 0.0 0.2 0.4 0.6 0.8 1.0 0 50 100 -4 -3 -2 -1 0 1 2 3 4 0.2 0.4 0.6 0.8 1.0 (b) T_{bath}= 0.1T_{c} h∗= 0.2∆∗ φ = π P_{I}(%) eV/∆∗ eV bi as / ∆∗ -100 -50 0 50 100 K_{coll} PI (%) (c) T_{bath}= 0.1T_{c} h∗= 0.2∆∗ φ = π eV = 1.0∆∗ eV_{bias}= 0.5∆∗
FIG. 14. 共Color兲 共a兲 Sketch of a possible setup for the imple-mentation of a spin-polarized current source. An additional super-conducting electrode 共S3兲 is coupled to the N region through a
tunnel junction of resistance Rp. The exchange fields in S1,2are
arranged in the antiparallel configuration. Spin-polarized current can be extracted by biasing the S3terminal with Vbias.共b兲 Contour
plot of the nonequilibrium current polarization P_{I}vs V and V_{bias}at
Tbath= 0.1Tc and h*= 0.2⌬*. 共c兲 PI vs Kcoll calculated eV = 1.0⌬* and eV_{bias}= 0.5⌬*for T_{bath}= 0.1T_{c}, h*= 0.2⌬*, and=.
have discussed the possibility of producing spin-polarized currents by coupling the N region to an additional supercon-ducting lead, finding that 100% spin polarization is realisti-cally achievable. This effect is fairly robust against the oc-currence of inelastic electron-electron collisions.
We shall finally comment on some possible applications of the structures presented here. An immediate first applica-tion of this system is the implementaapplica-tion of storage cell ele-ments, thanks to the very large TMR values关see Fig.8共a兲兴. Magnetic-field-controlled current switches can be envisioned as well关see Fig. 6共a兲兴. Importantly, power dissipation is in-trinsically limited owing to the small currents driven through NIS junctions. For example, assuming Rt= 103⍀ and
alumi-num共Al兲 electrodes at T=0.1Tc⬇0.12 K, a dissipated power
in the range of 10−15_{– 10}−12_{W can be achieved for 2共⌬}*
− h*兲/e⬍兩V兩 ⬍2⌬*/e. This makes this setup attractive for low-dissipation cryogenic applications. In light of a realistic implementation, ferromagnetic alloys such as Cu_{1−x}Nix共Ref. 53兲 or Pd1−xNix 共Ref. 54兲 共which allow fine tuning of h
through a proper choice of x兲 are promising candidates. For example, in Pd_{1−x}Nixalloy with x = 0.1, h⯝10 meV resulting
in F⬇5 nm.54 By choosing Al as S electrodes 关with ⌬
⯝200eV andS⬇300 nm 共Ref.55兲兴, it turns out that h*in
the range ⬃0.2⌬*– 0.5⌬* can be achieved. In such nano-structures, the bias voltage can be fed through outer normal metal electrodes, tunnel coupled to the ferromagnetic layers in order to prevent depolarization of the F electrodes. This would result in adding in series extra resistances which could be easily engineered in order to minimize the induced cor-rection to both tunnel magnetoresistance and operating volt-age.
ACKNOWLEDGMENTS
Partial financial support from the EU funded HYSWITCH, NanoSciERA “NanoFridge,” and RTNNANO projects is acknowledged.
1_{Theory of Nonequilibrium Superconductivity, edited by N. B.}
Kopnin共Clarendon, Oxford, 2001兲.
2_{P. Samuelsson, J. Lantz, V. S. Shumeiko, and G. Wendin, Phys.}
Rev. B 62, 1319共2000兲.
3_{H. Pothier, S. Guéron, N. O. Birge, D. Esteve, and M. H. Devoret,}
Phys. Rev. Lett. 79, 3490共1997兲.
4_{B. J. van Wees, K.-M. H. Lenssen, and C. J. P. M. Harmans, Phys.}
Rev. B 44, 470共1991兲.
5_{P. Samuelsson, V. S. Shumeiko, and G. Wendin, Phys. Rev. B 56,}
R5763共1997兲.
6_{V. S. Shumeiko, G. Wendin, and E. N. Bratus, Phys. Rev. B 48,}
13129共1993兲.
7_{L. Y. Gorelik, V. S. Shumeiko, R. I. Shekhter, G. Wendin, and M.}
Jonson, Phys. Rev. Lett. 75, 1162共1995兲.
8_{A. F. Volkov, Phys. Rev. Lett. 74, 4730}_{共1995兲.}
9_{A. F. Volkov and H. Takayanagi, Phys. Rev. B 56, 11184}_{共1997兲.} 10_{F. K. Wilhelm, G. Schön, and A. D. Zaikin, Phys. Rev. Lett. 81,}
1682共1998兲.
11_{S. K. Yip, Phys. Rev. B 58, 5803}_{共1998兲.}
12_{A. F. Morpurgo, T. M. Klapwijk, and B. J. van Wees, Appl. Phys.}
Lett. 72, 966共1998兲.
13_{J. J. A. Baselmans, A. F. Morpurgo, B. J. van Wees, and T. M.}
Klapwijk, Nature共London兲 397, 43 共1999兲.
14_{F. Giazotto, F. Taddei, T. T. Heikkilä, R. Fazio, and F. Beltram,}
Appl. Phys. Lett. 83, 2877共2003兲.
15_{F. Giazotto, T. T. Heikkilä, F. Taddei, R. Fazio, J. P. Pekola, and F.}
Beltram, Phys. Rev. Lett. 92, 137001共2004兲.
16_{F. Giazotto and J. P. Pekola, J. Appl. Phys. 97, 023908}_{共2005兲.} 17_{M. A. Laakso, P. Virtanen, F. Giazotto, and T. T. Heikkilä, Phys.}
Rev. B 75, 094507共2007兲.
18_{A. M. Savin, J. P. Pekola, J. T. Flyktman, A. Anthore, and F.}
Giazotto, Appl. Phys. Lett. 84, 4179共2004兲.
19_{J. P. Pekola, F. Giazotto, and O.-P. Saira, Phys. Rev. Lett. 98,}
037201共2007兲.
20_{O.-P. Saira, M. Meschke, F. Giazotto, A. M. Savin, M. Möttönen,}
and J. P. Pekola, Phys. Rev. Lett. 99, 027203共2007兲.
21_{J. P. Pekola, R. Schoelkopf, and J. Ullom, Phys. Today 57}_{共5兲, 41}
共2004兲.
22_{F. Giazotto, T. T. Heikkilä, A. Luukanen, A. M. Savin, and J. P.}
Pekola, Rev. Mod. Phys. 78, 217共2006兲.
23_{S. Takahashi, H. Imamura, and S. Maekawa, Phys. Rev. Lett. 82,}
3911共1999兲.
24_{S. Maekawa, S. Takahashi, and H. Imamura, J. Phys. D 35, 2452}
共2002兲.
25_{Y. Tserkovnyak and A. Brataas, Phys. Rev. B 65, 094517}_{共2002兲.} 26_{J. Johansson, V. Korenivski, D. B. Haviland, and A. Brataas,}
Phys. Rev. Lett. 93, 216805共2004兲.
27_{S. Takahashi, T. Yamashita, T. Koyama, and S. Maekawa, J. Appl.}
Phys. 89, 7505共2001兲.
28_{I. V. Bobkova and A. M. Bobkov, Phys. Rev. B 74, 220504}_{共R兲}
共2006兲.
29_{W. Belzig, A. Brataas, Yu. V. Nazarov, and G. E. W. Bauer, Phys.}
Rev. B 62, 9726共2000兲.
30_{F. Giazotto, F. Taddei, R. Fazio, and F. Beltram, Phys. Rev. Lett.}
95, 066804共2005兲.
31_{F. Giazotto, F. Taddei, R. Fazio, and F. Beltram, Appl. Phys. Lett.}
89, 022505共2006兲.
32_{See A. I. Buzdin, Rev. Mod. Phys. 77, 935}_{共2005兲; F. S. Bergeret,}
K. B. Efetov, and A. Volkov, ibid. 77, 1321共2005兲, and refer-ences therein.
33_{F. S. Bergeret, A. F. Volkov, and K. B. Efetov, Phys. Rev. Lett.}
86, 3140共2001兲.
34_{P. M. Tedrow and R. Meservey, Phys. Rev. Lett. 27, 919}_{共1971兲.} 35_{R. Meservey and P. M. Tedrow, Phys. Rep. 238, 173}_{共1994兲.} 36_{J. P. Pekola, T. T. Heikkilä, A. M. Savin, J. T. Flyktman, F. }
Gia-zotto, and F. W. J. Hekking, Phys. Rev. Lett. 92, 056804共2004兲.
37_{R. C. Dynes, J. P. Garno, G. B. Hertel, and T. P. Orlando, Phys.}
Rev. Lett. 53, 2437共1984兲.
38_{D. R. Heslinga and T. M. Klapwijk, Phys. Rev. B 47, 5157}
共1993兲.
Interac-tions in Disordered Systems, edited by A. L. Efros and M. Pollak
共Elsevier, Amsterdam, 1985兲.
40_{A. Kaminski and L. I. Glazman, Phys. Rev. Lett. 86, 2400}
共2001兲.
41_{A. Anthore, F. Pierre, H. Pothier, and D. Esteve, Phys. Rev. Lett.}
90, 076806共2003兲.
42_{K. E. Nagaev, Phys. Rev. B 52, 4740}_{共1995兲.}
43_{M. Yu. Kuprianov and V. F. Lukichev, Zh. Eksp. Teor. Fiz. 94,}
139共1988兲 关Sov. Phys. JETP 67, 1163 共1988兲兴.
44_{B. L. Altshuler and A. G. Aronov, Zh. Eksp. Teor. Fiz. 75, 1610}
共1978兲 关Sov. Phys. JETP 48, 812 共1978兲兴.
45_{A. Kamenev and A. Andreev, Phys. Rev. B 60, 2218}_{共1999兲.} 46_{B. Huard, A. Anthore, F. Pierre, H. Pothier, N. O. Birge, and D.}
Esteve, Solid State Commun. 131, 599共2004兲.
47_{M. Yu. Kupriyanov, A. Brinkman, A. A. Golubov, M. Siegel, and}
H. Rogalla, Physica C 326-327, 16共1999兲.
48_{M. Tinkham, Introduction to Superconductivity} _{共Dover, New}
York, 1996兲.
49_{F. J. Jedema, A. T. Filip, and B. J. van Wees, Nature}_{共London兲}
410, 345共2001兲.
50_{M. Johnson, Phys. Rev. Lett. 70, 2142}_{共1993兲.} 51_{T. T. Heikkilä, Ph.D. thesis, HUT Helsinki, 2002.} 52_{The constraint R}
pⰇRt ensures the nonequilibrium condition in the N region not to be appreciably perturbed by the current extraction from the superconducting terminal S_{3}.
53_{V. V. Ryazanov, V. A. Oboznov, A. Yu. Rusanov, A. V. }
Vereten-nikov, A. A. Golubov, and J. Aarts, Phys. Rev. Lett. 86, 2427 共2001兲.
54_{T. Kontos, M. Aprili, J. Lesueur, and X. Grison, Phys. Rev. Lett.}
86, 304共2001兲.
55_{J. Romijn, T. M. Klapwijk, M. J. Renne, and J. E. Mooij, Phys.}